Solid-state studies of phthalazinylhydrazones and triazolophthalazines: the role of the nitro group
Trzesowska-Kruszynska, Agata; CrystEngComm 17 (2015) 7702–; doi:10.1039/C5CE00846H

data_7222002
_publ_section_title
;
 Solid-state studies of phthalazinylhydrazones and triazolophthalazines:
 the role of the nitro group
;
_journal_issue                   40
_journal_name_full               CrystEngComm
_journal_page_first              7702
_journal_paper_doi               10.1039/C5CE00846H
_journal_volume                  17
_journal_year                    2015
_chemical_formula_moiety         'C17 H11 N5 O2'
_chemical_formula_sum            'C17 H11 N5 O2'
_chemical_formula_weight         317.31
_chemical_name_systematic
; 
3-[2-(4-nitrophenyl)ethenyl][1,2,4]triazolo[3,4-a]phthalazine
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_audit_update_record
;
2015-04-28 deposited with the CCDC.
2015-09-04 downloaded from the CCDC.
;
_cell_angle_alpha                75.576(14)
_cell_angle_beta                 87.07(2)
_cell_angle_gamma                68.757(17)
_cell_formula_units_Z            2
_cell_length_a                   6.9683(12)
_cell_length_b                   7.6250(17)
_cell_length_c                   14.408(3)
_cell_measurement_reflns_used    1305
_cell_measurement_temperature    100.0(1)
_cell_measurement_theta_max      50
_cell_measurement_theta_min      2
_cell_volume                     690.4(3)
_computing_cell_refinement       'SAINT-Plus (Bruker, 2009)'
_computing_data_collection       'APEX2 (Bruker, 2010)'
_computing_data_reduction        'SAINT-Plus (Bruker, 2009)'
_computing_molecular_graphics
;XP in SHELXTL/PC (Sheldrick, 2008)
 ORTEP-3 W v. 1.062 (Farrugia 2012)
;
_computing_publication_material
;SHELXL (Sheldrick, 2008) and
 PLATON (Spek, 2009)
;
_computing_structure_refinement  'SHELXL (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS (Sheldrick, 2008)'
_diffrn_ambient_temperature      100.0(1)
_diffrn_detector_area_resol_mean 12.8
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.848
_diffrn_measurement_device_type  'Bruker APEXII CCD area-detector'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         '30W microsource with MonoCap capillary'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0166
_diffrn_reflns_av_sigmaI/netI    0.0155
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            7768
_diffrn_reflns_theta_full        67.00
_diffrn_reflns_theta_max         84.08
_diffrn_reflns_theta_min         3.17
_diffrn_standards_decay_%        0.00
_diffrn_standards_interval_time  19.67
_diffrn_standards_number         8
_exptl_absorpt_coefficient_mu    0.872
_exptl_absorpt_correction_T_max  0.964
_exptl_absorpt_correction_T_min  0.870
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2003)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    1.526
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             328
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.273
_refine_diff_density_min         -0.294
_refine_diff_density_rms         0.053
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.056
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     217
_refine_ls_number_reflns         2625
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.056
_refine_ls_R_factor_all          0.0362
_refine_ls_R_factor_gt           0.0348
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0583P)^2^+0.2448P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0959
_refine_ls_wR_factor_ref         0.0991
_reflns_number_gt                2491
_reflns_number_total             2625
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5ce00846h2.cif
_cod_data_source_block           con83a
_cod_depositor_comments
'Adding full bibliography for 7221992--7222004.cif.'
_cod_original_cell_volume        690.4(2)
_cod_database_code               7222002